Two magnetic phase transitions, driven by symmetry breaking and isostructural phase transitions, in a nickel-bis-dithiolene spin system
Ning, Wei-Hua; Chen, Xuan-Rong; Liu, Jian-Lan; Guo, Ping-Chun; Ren, Xiao-Ming; New Journal of Chemistry 38 (2014) 179–; doi:10.1039/c3nj01101a

data_7053952
_publ_section_title
;
 Two magnetic phase transitions, driven by symmetry breaking and
 isostructural phase transitions, in a nickel-bis-dithiolene spin system
;
_journal_issue                   1
_journal_name_full               'New Journal of Chemistry'
_journal_page_first              179
_journal_paper_doi               10.1039/c3nj01101a
_journal_volume                  38
_journal_year                    2014
_chemical_formula_sum            'C16 H5 D6 N6 Ni S4'
_chemical_formula_weight         480.29
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.912(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.9131(8)
_cell_length_b                   17.7611(19)
_cell_length_c                   14.9879(18)
_cell_measurement_temperature    296(2)
_cell_volume                     2075.0(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0707
_diffrn_reflns_av_sigmaI/netI    0.0673
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            28961
_diffrn_reflns_theta_full        27.49
_diffrn_reflns_theta_max         27.49
_diffrn_reflns_theta_min         1.79
_exptl_absorpt_coefficient_mu    1.351
_exptl_crystal_density_diffrn    1.537
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             964
_refine_diff_density_max         0.854
_refine_diff_density_min         -0.439
_refine_diff_density_rms         0.101
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.999
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     244
_refine_ls_number_reflns         4739
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.999
_refine_ls_R_factor_all          0.1512
_refine_ls_R_factor_gt           0.0619
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0953P)^2^+1.0367P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1549
_refine_ls_wR_factor_ref         0.1955
_reflns_number_gt                2300
_reflns_number_total             4739
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3nj01101a.txt
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      P21/n
_cod_database_code               7053952